Structural Classification of Basalt FRP at High Temperatures

Department of Civil Engineering, Vignan’s Institute of Information Technology (A), Duvvada, Visakhapatnam 530049, India Department of Civil Engineering, Gayatri Vidya Parishad, Rushikonda, Visakhapatnam 530045, India Department of Civil Engineering, Gayatri Vidya Parishad College of Engineering (A), Madhurawada, Visakhapatnam 530048, India Department of Chemical Engineering, College of Biological and Chemical Engineering, Addis Ababa Science and Technology University, Addis Ababa, Ethiopia


Introduction
Ductility is the capacity of a structural member to undertake large inelastic deformations without notable loss of strength or stiffness. Due to ductility, structures or materials can absorb energy by deforming into an inelastic range under the application of force. In other words, it is the ability to withstand plastic deformation before fracture which can be defined as the ratio of the ultimate deformation at an assumed collapse point to the yield deformation. For resistance to earthquake forces, the structure, elements, and connections shall be designed to have ductile failure to avoid sudden collapse. However, ductility is hard to achieve in many structural members such as deep beams, pile caps, and corbels. Since such members tend to fail mostly in the shear mode, the assumptions of the linearelastic flexural theory and pure bending theory are not valid. ese members require special considerations for design and detailing. erefore, in order to achieve ductility, many design methodologies like Strut-and-Tie model and materials such as admixtures, plasticizers, and fibers are adopted. Moreover, with the increase in fire-related disasters around the world, the importance of fire-resistant construction is escalating. In recent decades, many researchers [1][2][3][4][5][6][7][8][9][10][11] have studied the properties and applicability of basalt fiber in structural members due to its high temperature resistance, high durability, high elastic strength, sustainability, etc. It has been found that satisfactory mechanical and thermal-resistant properties of structural members can be achieved using chopped basalt fibers, basalt fiber-reinforced polymer (BFRP) bars, BFRP sheets, laminates, etc. However, contradictory findings are also available in the literature regarding the residual mechanical strength of basalt fibers subjected to elevated temperature conditions. erefore, in this work, an attempt has been made to study the mechanical properties of basalt fibers subjected to various temperature conditions. e chopped fibers could not be tested directly due to the smaller lengths, for which laminates are prepared to test the mechanical properties as per ASTM standards. e basalt fiber samples were elevated to different temperatures, and then, through mechanical testing, the residual stress of fibers was evaluated and compared. erefore, in recent times, the basalt fibers are of importance in research because of its high mechanical properties, thermal resistance, durability, sustainability, low production cost, etc. Basalt filaments are formed by melting the basalt rock which passes through orifices and pullers over a roller [12]. e economic advantage, lower environmental impact, and higher mechanical strength are achieved because no additives are required to produce these fibers from high-strength basalt rocks. e authors of [12,13] found that volcanic magma crystallizes to basalt with very low water content at the time of crystallization. Basalt rocks are the partial melting products of primitive rocks such as garnet peridotite. Basalt consists of minerals such as plagioclase and clinopyroxene along with olivine, nepheline, melilite, hypersthene, quartz, etc. Based on the original rock used, the produced fibers may exhibit different mechanical and chemical properties. Soares et al. [14] stated that acidic basalt which contains more than 46% of SiO 2 is suitable for production of basalt fiber because in order to develop glass network, high silica content is necessary. As stated earlier, basalt fibers are available with different chemical compositions containing 51.56-57.5% SiO 2 , 16.9-18.2% Al 2 O 3 , 5.2-7.8% CaO, 1.3-3.7% MgO, 2.5-6.4% Na 2 O, 0.8-4.5% K 2 O, 4.0-9.5% Fe 2 O 3 , etc.
Investigation was performed on temperature resistance of basalt fibers which generally has an operational temperature range from −200°C to 800°C [15]. Basalt fibers perform much better than glass fibers as the temperature range of basalt fibers is −269°C to 700°C as compared to glass fibers whose temperature range is from −60°C to 500°C [16]. Most of the studies show that basalt fibers perform very efficiently at high temperatures. However, contradictory results are found in different literature studies regarding the residual mechanical strength of basalt fibers subjected to elevated temperature conditions. e authors of [16] found that with the increase of time of exposure and elevated temperature up to 300°C, the strength of basalt fibers increased up to 19.1%. Also, 32.8% reduction of strength is observed in similar testing conditions [17]. Zollo et al. [16] explained that the reformation of fiber structure around the nucleating agents led to the thermal stability of the fibers. However, Arvo Ivar and Bjorklund [17] described from SEM and XRD analysis that the short-order structure of basalt fibers decreased in size which led to reduction in tensile strength. A lot of research was performed on functionally graded hybrid composite materials, and parametric study has also been performed on these novel layups [18][19][20][21][22]. is layup can be applied in case of basalt fibers also. erefore, it is necessary to analyze residual mechanical strength of the basalt fiber specimens subjected to elevated temperatures because such variations occur due to the change in the crystalline structure of the fiber which is mainly governed by the presence of iron oxides.

Tensile Properties of BFRP Specimens.
e in-plane tensile properties of polymer matrix composite materials reinforced with high-modulus fibers can be determined as per ASTM D 3039/D3039M [23]. Monotonically tensile load is applied on the flat strip of the material with a constant rectangular cross section which is mounted in the grips as shown in Figure 1.
e maximum load carried before failure is the ultimate failure strength of the material. Moreover, if the strain or displacement is monitored, then stress-strain response can be obtained. e speed of test should be controlled at a constant head displacement rate of 2 mm/min or a standard strain rate of 0.01 min −1 .

Flexure Properties of BFRP Specimens.
Basalt fiberreinforced polymer (BFRP) specimens were subjected to flexural load under the three-point bending system as shown in Figure 2. Both rigid and semirigid materials in the shape of rectangular bars moulded directly or machined from plates, sheets, or moulded shapes can be tested within the 5% strain limit of the test methods [1].
As shown in Figure 2, a bar of rectangular cross section resting on two supports is loaded at midway where the radius of the support is of minimum 3.2 mm to maximum 1.6 times the specimen depth, whereas the maximum radius of the loading nose is limited to 4 times the specimen depth. e support span-to-depth ratio of 16 : 1 should be maintained at a strain rate of 0.01 mm/mm/min. e failure occurs at a maximum strain of 5%. e rate of crosshead motion is determined using the following equation: e flexural strength, chord, secant, or tangent modulus of elasticity and the total work can be measured by calculating the area under the load-deflection curve. If "r" is the strain in mm/mm, the mid-span deflection (D) can be calculated using the following equation:

Basalt Fibers.
Basalt fibers were acquired from Go Green Products, Chennai, which were of 24 mm length and diameter more than 5 microns (Go Green Products 2018). As per the supplier, the density was 2.6 g/cm 3 , melting point was 1450°C, and they constituted odorless golden shine fibers ( Figure 3). eir chemical composition is shown in Table 1.

2
Advances in Materials Science and Engineering

Epoxy and
Hardener. An epoxy resin of grade "Resin 691" and a hardener of grade "Reactive Polyamide 140" have been used. e ratio of the resin to hardener is maintained at 9 : 1 by weight [24]. e mechanical properties of the resin are given in Table 2.
e thermal properties of the basalt fiber are significant in the current study. Hence, the properties are depicted in Table 3.

Specimen Preparation
As per ASTM D3039/D3039M [3], five basalt fiber-reinforced (BFRP) specimens of uniform geometry should be prepared. e geometry depends on fiber orientation, gage length, grip type and length, use of tab, etc. At three places in the gage section, width (w) and thickness (h) are calculated to find the average cross-section area (A) from the following equation: e laminates of size 310 × 310 × 2.5 ± (0.15) mm (length × width × thickness) are prepared in the mould developed at Advanced Composites Laboratory, BITS, Pilani. e mechanical properties of basalt fibers are characterized by subjecting them to elevated temperatures of 300°C and 600°C. Initially, the fibers are kept in an electric muffle furnace as shown in Figure 4(a), and the fibers are removed after heating, as shown in Figure 4(b). e mould of heavy flat metal base plates is used to apply uniform pressure to prepare the laminates, flat aluminum sheets are used for smooth surface finishing, and the outer rectangular blockboard ring is used to maintain the dimension of the laminates, as shown in Figure 5. e matrix consists of the epoxy resin of grade "Resin 691" along with the hardener "Reactive Polyamide 140" at the ratio of 9 :1 by weight. e ratio of the fiber to matrix is maintained as 0.6. Since the glass transition temperature of the resin is 91.23°C and decomposition temperature is 230°C only, the laminates are not tested at    Advances in Materials Science and Engineering elevated temperatures but only the residual stress of fibers are calculated by preparing the laminates using the resin and hardener. Even though many attempts were made to prepare linearly oriented fiber-reinforced composite plates, due to the smaller length of the fiber and dispersion of epoxy resin, the orientation of fibers in the laminates was considered as randomly distributed. After mixing the fibers with the matrix, the plates are tightened using screws and kept for minimum 40 hours of conditioning. After proper conditioning of the laminates, specimens are prepared by cutting using a DoAll cutting machine at Mechanical Workshop, BITS, Pilani, as shown in Figure 6. e tensile specimens of size 250 × 25 × 2.5 mm (length × width × thickness) are considered as per Table 2 of ASTM D 3039/D 3039M, and flexure specimens of size 12.7 × 2.5 mm (width × thickness) with varying lengths are used to accommodate at least 10% overhanging after maintaining 16 : 1 span-to-depth ratio conforming to ASTM D790 [25].
ree types of specimens have been prepared in this study. One with fibers without any temperature treatment, other with fibers subjected to 300°C elevated temperature, and the last with fibers subjected to 600°C elevated temperature.
ese three specimens are named as BFRP-I, BFRP-II, and BFRP-III, respectively. Laminates are machined, and all the 5 specimens (both for tensile and flexural tests) are depicted in Figure 7.
e coefficient of variation of the tensile and flexural stress of the specimens tested has been calculated using equation (4) to maintain the quality of work done. e coefficient of variation for all the specimens is not greater than 10% which is considerable:

Results and Discussion
e BFRP specimens are tested, and the results are discussed as follows.

Tensile Behavior.
e failure of the BFRP specimen tested in a universal testing machine is shown in Figure 8. e type of failure observed was lateral gage middle (LGM) LGM failure Advances in Materials Science and Engineering failure since the crack appeared laterally at the mid-position of the specimen. A similar type of failure was observed in all the specimens tested under tensile load. e stress-strain graphs of BFRP-I, BFRP-II, and BFRP-III are depicted in Figure 9, and the bar charts representing the maximum stress obtained and the maximum strain obtained at peak stress are also shown in Figure 12.
BFRP-I has obtained the highest tensile stress among other specimens subjected to elevated temperature. It is worth noting that specimens elevated at 600°C have the least tensile stress. Surface fractured at the soffit of the specimen

Advances in Materials Science and Engineering
Hence, it is observed that increase in tensile stress is observed until 300°C temperature. Further increase in temperature leads to decrease in tensile stress. Although the stress is low, temperature-elevated specimens exhibit ductile nature; i.e., the failure of the specimens is not catastrophic.

Flexural
Behavior. e specimens are tested under a three-point bending apparatus as shown in Figure 10. e soffit of the specimen was fractured upon the application of load at the middle as shown in Figure 10.
e flexural stress-strain graphs are plotted in Figure 11. It is observed that BFRP-I, i.e., the specimen without temperature curing, obtained the highest flexural stress among other specimens. e BFRP-II specimen has higher flexural stress than the BFRP-III specimen. A similar trend has been observed in the case of tensile specimens. As shown in Figures 12 and 13, the residual tensile stress of basalt fibers elevated to 300°C is around 84%, whereas for 600°C, it is around 13% of maximum stress. However, the strain at maximum stress shows that ductile behavior of the specimen is maintained even at 600°C which signifies that even at higher temperature, the fibers perform quite well in case of serviceability. e reduction of stress due to higher temperature may not be due to change in the crystalline structure of the fibers but also due to poor interlaminar shear strength. e specimens are ductile in nature since none of the specimens collapsed suddenly (see Figures 9 and 11).
Particularly, in comparison with the tensile results, it was discovered that the residual stress of flexure basalt fibers elevated at 300°C is approximately 54% of the maximum stress, while it is approximately 10% of the maximum stress in the case of fibers elevated at 600°C. e current study's structural applications are diverse. e laminates made of basalt fiber can be used as a direct material or as a retrofitting material. Roof panels, pultruded beams, load bearing I-sections, partition members, pedestrian bridges, railway sleepers, and other structural members made of basalt fibers can be used directly. e basalt fibers can be utilized for column wrapping and slab strengthening by connecting the fiber sheet at the soffit and as near surface mounted members in the case of retrofitting technique. e following are some of the applications for basalt fiberreinforced polymer laminates. e added benefit of this material, in particular, is that it is thermally resistant.

Conclusions
e following conclusions are made from this study: (1) Basalt fiber has high tensile strength and modulus of elasticity, making it suitable for use in reinforced composites. (2) e electrical insulation of basalt fiber is greater than that of glass fiber. (3) e electromagnetic wave has excellent permeability; if a basalt fiber cloth is added to the building's wall, it can produce good shielding for all types of electromagnetic waves. (4) e residual stress of basalt fiber decreases, as the temperature increases in case of both tensile and flexural specimens irrespective of time. (5) e experiment shows the sustainability and reusability of basalt fiber since at higher temperature, the ductile behavior is maintained and residual stress up to 300°C is still satisfactory. (6) With the use of high-temperature-resistant epoxy resin, basalt fibers can be used in fire-resisting constructions very effectively. (7) Excellent compatibility with metal, plastic, carbon fiber, and other materials is found. Also, the composite of basalt continuous fiber and various types of resin has a stronger bonding strength than of glass fiber and carbon fiber. In terms of strength, composites made of continuous basalt fiber are equivalent to E-glass fiber, but elastic modulus has obvious advantages in all types of fibers.

Data Availability
e data used to support the findings of this study are included within the article.

Disclosure
is study was performed as part of the employment at Addis Ababa Science and Technology University, Addis Ababa, Ethiopia.